Low dimensional solids based on Mo6 cluster cyanides and Mn2+, Mn3+ or Cd2+ metal ions: crystal chemistry, magnetic and optical properties
Daigre, Gilles; Lemoine, Pierric; Pham, Thi Diep; Demange, Valérie; Gautier, Régis; Naumov, Nikolay G.; Ledneva, Alexandra; Amela-Cortes, Maria; Dumait, Noée; Audebrand, Nathalie; Cordier, Stéphane; CrystEngComm 20 (2018) 3396–; doi:10.1039/C8CE00113H

data_7230698
_publ_section_title
;
 Low dimensional solids based on Mo6 cluster cyanides and Mn2+, Mn3+ or
 Cd2+ metal ions: crystal chemistry, magnetic and optical properties
;
_journal_issue                   24
_journal_name_full               CrystEngComm
_journal_page_first              3396
_journal_paper_doi               10.1039/C8CE00113H
_journal_volume                  20
_journal_year                    2018
_chemical_formula_sum            'C6 Br8 Fe Mo6 N6 O2'
_chemical_formula_weight         1458.89
_space_group_crystal_system      orthorhombic
_space_group_IT_number           74
_space_group_name_Hall           '-I 2b 2'
_space_group_name_H-M_alt        'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_audit_creation_method           SHELXL-2017/1
_audit_update_record
;
2017-10-05 deposited with the CCDC.
2018-05-21 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   19.473(4)
_cell_length_b                   10.3173(17)
_cell_length_c                   13.749(3)
_cell_measurement_reflns_used    4815
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      27.53
_cell_measurement_theta_min      2.47
_cell_volume                     2762.3(9)
_computing_cell_refinement       'APEX2 (Bruker, 2014); SAINT (Bruker, 2014)'
_computing_data_collection
'SAINT (Bruker, 2014); XPREP (Sheldrick, 2014)'
_computing_data_reduction
'SAINT (Bruker, 2014); XPREP (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector                 '(CMOS) PHOTON 100'
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.945
_diffrn_measurement_device_type  'D8 VENTURE Bruker AXS'
_diffrn_measurement_method       'rotation images'
_diffrn_radiation_monochromator  'multilayer monochromator'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'Incoatec microfocus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0564
_diffrn_reflns_av_unetI/netI     0.0562
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.945
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            5410
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.945
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.547
_diffrn_reflns_theta_min         2.234
_exptl_absorpt_coefficient_mu    14.733
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.4679
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
  [Sheldrick, G.M. (2014). SADABS Bruker AXS Inc., Madison, Wisconsin, USA]
;
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.508
_exptl_crystal_description       plate
_exptl_crystal_F_000             2608
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_refine_diff_density_max         7.217
_refine_diff_density_min         -6.091
_refine_diff_density_rms         1.040
_refine_ls_extinction_coef       0.0006(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_goodness_of_fit_ref   1.116
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     68
_refine_ls_number_reflns         1761
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.116
_refine_ls_R_factor_all          0.1789
_refine_ls_R_factor_gt           0.1526
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1803P)^2^+2961.3667P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.4307
_refine_ls_wR_factor_ref         0.4529
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1412
_reflns_number_total             1761
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8ce00113h2.cif
_cod_data_source_block           shelx_CCDC3
_cod_depositor_comments
'Adding full bibliography for 7230695--7230700.cif.'
_cod_original_cell_volume        2762.3(8)
_cod_database_code               7230698
_shelx_shelxl_version_number     2017/1
_shelx_res_checksum              40417